A zoom into the nanoscale texture of secondary cell walls
- 8.6k Downloads
Besides classical utilization of wood and paper, lignocellulosic biomass has become increasingly important with regard to biorefinery, biofuel production and novel biomaterials. For these new applications the macromolecular assembly of cell walls is of utmost importance and therefore further insights into the arrangement of the molecules on the nanolevel have to be gained. Cell wall recalcitrance against enzymatic degradation is one of the key issues, since an efficient degradation of lignocellulosic plant material is probably the most crucial step in plant conversion to energy. A limiting factor for in-depth analysis is that high resolution characterization techniques provide structural but hardly chemical information (e.g. Transmission Electron Microscopy (TEM), Atomic Force Microscopy (AFM)), while chemical characterization leads to a disassembly of the cell wall components or does not reach the required nanoscale resolution (Fourier Tranform Infrared Spectroscopy (FT-IR), Raman Spectroscopy).
Here we use for the first time Scanning Near-Field Optical Microscopy (SNOM in reflection mode) on secondary plant cell walls and reveal a segmented circumferential nanostructure. This pattern in the 100 nm range was found in the secondary cell walls of a softwood (spruce), a hardwood (beech) and a grass (bamboo) and is thus concluded to be consistent among various plant species. As the nanostructural pattern is not visible in classical AFM height and phase images it is proven that the contrast is not due to changes in surfaces topography, but due to differences in the molecular structure.
Comparative analysis of model substances of casted cellulose nanocrystals and spin coated lignin indicate, that the SNOM signal is clearly influenced by changes in lignin distribution or composition. Therefore and based on the known interaction of lignin and visible light (e.g. fluorescence and resonance effects), we assume the elucidated nanoscale structure to reflect variations in lignification within the secondary cell wall.
KeywordsSecondary cell walls Scanning near field optical microscopy Atomic force microscopy Diffraction limit Lignification
Atomic Force Microscopy
Fourier Transform Infra-Red Spectroscopy
Scanning Near-Field Optical Microscopy
Transmission Electron Microscopy.
Structure, chemistry and mechanics of the polymer assembly of secondary cell walls have been studied for decades, because of the high social, environmental and economic relevance of the plant material in classical applications (e.g. wood, paper). More recent research activities are driven by the utilization of lignocellulosic biomass for bioenergy [1, 2, 3] and novel biomaterials . The organization of secondary cell walls at the micro-level, with its three-layered and multilamellar structure for wood species and bamboo respectively, is well understood. However we are still lacking knowledge on the organization at the nanoscale in particular about the spatial arrangement and interaction of the different polymers within the cell wall. Most secondary cell walls of xylem cells are made up of the three dominating cell wall polymers cellulose, lignin and hemicelluloses. Cellulose fibrils with a diameter of 3-4 nm are arranged in bigger agglomerates (fibril bundles) with a size of 20-25 nm and are embedded in a matrix consisting of lignin and hemicelluloses [5, 6]. During the last decades different cell wall models on the spatial arrangement of the macromolecules within the secondary cell walls have been developed. The micellar theory of Nägeli  (developed in the 19th century) refers to a spatial distribution of the macromolecules in a concentric lamellae structure due to alternating circumferential layers of higher cellulose and higher lignin content. This theory has been supported in various studies based on visible/ultraviolet microscopy, the delamination behavior of wood fibers, the distribution and form of pores after selective removal of lignin as well as electron microscopy and atomic force microscopy studies [8, 9, 10, 11]. A slightly different model was supposed by Kerr and Goring  in terms of concentric arrangement of batches of higher cellulose and lignin content resulting in a segmented lamella structure. Based on high resolution field emission scanning electron microscopy studies on fractured wood samples and cell wall degradation by fungi, an alternative radial agglomeration of cellulose structures was proposed [13, 14]. More recently, electron microscopy and atomic force microscopy (AFM) studies supported a random texture without any structured arrangement of the wood components [15, 16].
All introduced models are mainly based on electron microscopy studies [11, 12, 14, 17] or on AFM experiments [5, 9, 10, 16]. Both methods are excellent in providing structural information with high resolution, but their potential to provide chemical information is quite limited. Alternative techniques that are strong in chemical analysis of cell walls such as Raman spectroscopy  are limited in the required spatial resolution due to the diffraction limit (Rayleigh criterion). To probe structure and chemistry on the nano-level at the same time, scanning probe microscopy has to be combined with spectroscopic techniques [19, 20]. One possible combination is Scanning Near-Field Optical Microscopy (SNOM), which has already been developed in the late nineteen-twenties based on the first considerations on breaking the diffraction limit in microscopy . A sample is scanned by a gold or silver coated optical tip, into which a laser is coupled in, with a subwavelength aperture at the end of the optical fiber. The generated signal is not affected by the constraints of diffraction and provides additional photo-optical and thus chemical information. It is based on evanescent waves, which are characterized by rapidly decaying amplitudes very close to the surface (nm range) [22, 23, 24]. Although SNOM has been used for the characterization of various biological samples such as proteins, lipids, polysaccharides, DNA and cells [25, 26], intact secondary plant cell walls have not been analyzed yet. Therefore the aim was to reveal new insights into the chemical structure of secondary plant cell walls with the help of Scanning Near Field Optical Microscopy by zooming into the nanoscale texture of cell walls of a hardwood, a softwood and a grass.
Results and discussion
Figure 4c shows the topography of the self-assembled lignin model compounds on top of the cellulose nanocrystal film. The images indicate that the lignin forms globular structures (bigger z-range compared to Figure 4b) in the size of 250-500 nm on top of the cellulose nanocrystals which is in good agreement with the results of previous publications [27, 28, 29]. Remarkably, the underlying structure of the cellulose nanocrystals is still visible. In contrast, the SNOM image of the bilayer (Figure 4d) reveals only the individual globules of lignin macromolecules and their agglomerations.
The SNOM images provide for the first time sub-diffraction limited chemical information on the spatial distribution of the cell wall components in secondary cell walls. The circumferential pattern of cellulose and lignin rich regions is likely to be the result of spatial constraints and progression of the cell wall formation process. The superimposed circumferential structure is due to the cellulose fibril spinning process by cellulose synthase complexes , which lay down the cellulose scaffold in a circumferential manner. The subsequent lignification in a radical polymerization process is likely to locally produce segments of higher and lower degrees of lignin or alterations in the chemical structure [35, 36, 37], which become evident in the SNOM images. A striking observation is the incidence of the distribution pattern among different plant species, including a representative of hardwoods, softwoods and grasses. This points to a rather universal principle of spatial cellulose and lignin assembly in secondary cell walls, and is therefore highly relevant for the understanding of cell wall structure and its enzymatic degradation for energy conversion from lignocellulosic raw materials in general.
Air dried specimens of spruce, beech (provided by Oliver Vay, Kompetenzzentrum Holz GmbH, Linz, Austria) and bamboo (from an experimental forest in Miaoshanwu Nature Reserve, Zhejiang Province, China) with dimensions of ~10×10×10 mm3 (radial/tangential/longitudinal) were glued onto AFM specimen discs (orientation of the fibrils was taken into account) and afterwards on cylinders due to fixation reasons. A highly smooth surface (1.5 × 1.5 mm2) was cut using a ultramicrotome (Reichert Jung–Ultracut) with a diamond knife (DiATOME) and the following cutting parameters: speed: 1 mm/s, clearance angle: 8° and cutting angle: 45°. Sections of initially 2 μm reduced gradually to approximately 50 nm were removed in order to minimize mechanical impact of cutting forces on the surface. Both, wood (beech and spruce) and bamboo samples were not embedded, to avoid any potential influence by the embedding material.
Cellulose nano-crystals (CNCs) were prepared from ramie (Boehmeria nivea) fibers and synthetic lignins (Dehydrogenation Polymers - DHP) were synthetisized by peroxidase/hydrogen peroxide mediated polymerization of coniferyl alcohol (guaiacyl G unit), as previously described . 200 μg of CNC was applied to a clean quartz slide (3.14 cm2) from CNC aqueous suspension (0.1%, w/v) and dried under vacuum for 12 h. DHP solution (2 gL-1) in dioxan/water (9/1, v/v) was then deposited by spin-coating on CNC film with a spin-coater (Speedline Technologies, USA). A volume of 50 μL was deposited on a stationary solid slide, which was then accelerated at 1260 rpm/s and spun at 3000 rpm for 40 s. Thickness and refractive index of CNC film before DHP deposit were respectively 270 nm ± 5 nm and 1.550, measured by spectroscopic ellipsometry (Uvisel, Horiba Jobin Yvon, Palaiseau, France).
Size of the generated AFM/SNOM images varies between 20 × 20 μm2- 2.5 × 2.5 μm2 at a resolution of 256 × 256 pixels and 12 sub-steps between each pixel. Further information on the spatial resolution of the SNOM and AFM mode of the instrument can be found on http://www.nanonics.co.il. For processing the acquired data were exported from the measurement software (Quartz, Faraday Instruments) to WSxM 4.0 develop 11.6 software. All images were parabola flattened, equalized and the contrast was adjusted for visibility reasons .
We thank the SNF for funding in the framework of R’Equip and NRP66, as well BAFU (Bundesamt für Umwelt) and Lignum, Switzerland for the support of the Wood Materials Science professorship. Johannes Konnerth acknowledges the financial support for the STSM at ETH by COST Action FP0802. Correspondence and requests for materials should be addressed to I.B. (email@example.com).
- 7.Nägeli C: Die Micellartheorie. 1928, Leipzig: Akademische Verlagsgesellschaft M.B.HGoogle Scholar
- 12.Kerr AJ, Goring DAI: The Ultrastructural Arrangement of the wood cell wall. Cellul Chem Technol. 1975, 9: 563-573.Google Scholar
- 20.Yarbrough JM, Himmel ME, Ding SY: Plant cell wall characterization using scanning probe microscopy techniques. Biotechnol Biofuels. 2009, 2:Google Scholar
- 25.Lewis A, Taha H, Strinkovski A, Manevitch A, Khatchatouriants A, Dekhter R, Ammann E: Near-field optics: from subwavelength illumination to nanometric shadowing. Nat Biotechnol. 2003, 21: 1377-1386.Google Scholar
- 29.Micic M, Jeremic M, Radotic K, Leblanc RM: A comparative study of enzymatically and photochemically polymerized artificial lignin supramolecular structures using environmental scanning electron microscopy. J Colloid Interface Sci. 2000, 231: 190-194. 10.1006/jcis.2000.7136.CrossRefPubMedGoogle Scholar
- 37.Joseleau JP, Ruel K: Study of lignification by noninvasive techniques in growing maize internodes - An investigation by Fourier transform infrared cross-polarization magic angle spinning C-13-nuclear magnetic resonance spectroscopy and immunocytochemical transmission electron microscopy. Plant Physiol. 1997, 114: 1123-1133. 10.1104/pp.114.3.1123.PubMedCentralCrossRefPubMedGoogle Scholar
- 38.Horcas I, Fernandez R, Gomez-Rodriguez JM, Colchero J, Gomez-Herrero J, Baro AM: WSXM: a software for scanning probe microscopy and a tool for nanotechnology. Rev Sci Instrum. 2007, 78:Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.